## Hybrid Lattice Boltzmann/Dynamic Self-Consistent

## Field Simulations of Microphase Separation and Vesicle

## Formation in Block Copolymer Systems

*Liangshun Zhang1*, Agur Sevink2+, and Friederike Schmid3* *

*_{Institute of physics, Johannes Gutenberg Universität Mainz, D-55099 Mainz, Germany }
+_{Leiden Institute of Chemistry, Universiteit Leiden, 2300 RA Leiden, Niederlande }

We present a hybrid numerical method to introduce hydrodynamics in dynamic self-consistent field (SCF) studies of inhomogeneous polymer systems. It solves a set of coupled dynamical equations: The Navier-Stokes equations for the fluid flow, and SCF-based convection-diffusion equations for the evolution of the local monomer compositions. The Navier-Stokes equations are simulated by the lattice Boltzmann method and the dynamic self-consistent field equations are solved by a finite difference scheme. Two applications are presented: First, we study microphase separation in symmetric and asymmetric block copolymer melts with various values of shear and bulk viscosities, comparing the results to those obtained with purely diffusive dynamics. Second, we investigate the effect of hydrodynamics on vesicle formation in amphiphilic block copolymer solutions. In agreement with previous studies, hydrodynamic interactions are found to have little effect on the microphase separation at early times, but they substantially accelerate the process of structure formation at later times. Furthermore, they also contribute to selecting the pathway of vesicle formation, favoring spherical intermediates over aspherical (disklike) ones.

1_{ E-mail: shunshun122@gmail.com }
2_{ Email: a.sevink chem.leidenuniv.nl }

3_{ Corresponding Author: E-Mail: Friederike.Schmid@Uni-Mainz.DE }

**1. INTRODUCTION **

Block copolymers, where chemically distinct building blocks are connected by covalent bonds, can spontaneously self-assemble into a variety of nanoscale ordered microstructures. For example, melts of block copolymers may organize themselves as lamellae, cylinders, spheres, or complex bicontinuous structures. 1 , 2 Amphiphilic block copolymers in solution 3,4 may self-assemble into, e. g., spherical and cylindrical micelles, bilayer membranes, and vesicles. These microstructures can be tailored by varying the copolymer composition and segregation degree between the two blocks and have attracted widespread interests in both fundamental and technological contexts.

During the formation of ordered microstructures following a quench, the long-range hydrodynamic interactions strongly influence the domain

coarsening.5 This can already be observed in simple
binary mixture.6,7,8,9_{ Theories as well as numerical }

simulations of spinodal decomposition of binary mixture show that domains grow according to a power law behaviour and the growth exponent is a universal constant, which is different for systems with and without hydrodynamic interactions. For more complex systems, the effect of hydrodynamic effects on phase ordering and coarsening is less clear. A general feature seems to be that hydrodynamic flows speed up the coarsening process and help to prevent trapping in metastable states.

introduced by a velocity field, which is defined in terms of a vertical vorticity. The calculations indicate that the hydrodynamic flows are effective in the ordering process of symmetric block copolymers, while they are not important for the asymmetric block copolymers. Going beyond cell dynamics, the Lattice Boltzmann (LB) method has emerged as a powerful tool to solve the Navier-Stokes equations on a lattice.18 , 19 Phase separation and interface dynamics can be incorporated into the LB method either directly by introducing intermolecular interactions, or via free energy functional based concepts, or using other mesoscopic equations.12, 20 , 21 , 22 , 23 , 24 . The LB method is computationally efficient and comparatively easy to parallelize for large size simulations. Gonnell, Xu and co-workers have combined the LB method with a time-dependent Ginzburg-Landau model to study microphase separation in block copolymers.12,13,14,15 The approach deals with hydrodynamic interaction, but does not explicitly take into account the conformational entropy of polymer chains.

On the other hand, polymer-specific dynamic
models like the dynamic self-consistent field (SCF)
theory are becoming increasingly popular for
studying kinetic processes in inhomogeneous
polymer systems. 25 , 26 , 27 , 28 , 29 Unlike
phenomenological Ginzburg-Landau theories, the
SCF theory accounts for the chain connectivity and
provides a unified treatment of polymer systems in
intermediate and strong segregation regions.30 , 31
However, the dynamics in most dynamic SCF
simulation methods is purely diffusive and does not
account for hydrodynamic effects. A few efforts have
been made in recent years to overcome this drawback.
Maurits et al. have devised a hydrodynamic SCF
approach which combines the dynamic SCF
equations with a simple hydrodynamic model based
on the Darcy’s law for permeable media, i.e.,
hydrodynamic interactions were assumed to be
purely local. This approach was used to examine the
influence of hydrodynamic flows on the evolution
process of microstructures.32_{ Already at this level, }

the convective flows were found to accelerate domain growth and the removal of defects in the late stage of ordering. Honda and Kawakatsu combined dynamic SCF theory with the Navier-Stokes equations to investigate the hydrodynamic effects on the disorder-to-order transition of block copolymers. 33 A quasistatic approximation was developed to solve the Navier-Stokes equations.

They found that a system with lower viscosity has a lower free energy density. Song et al. combined a dynamic SCF approach with the lattice Boltzmann method to study the effects of hydrodynamic interactions on the microphase separation process of block copolymers and defect evolution of lamellar microstructures in two-dimensional space.23,24 In their method, the convection-diffusion equation for the evolution of the order parameter is numerically solved by the lattice Boltzmann method, which may generate unphysical flows due to spurious terms.34 Hall et al. have developed a complex framework named hydrodynamic self-consistent field theory (HSCF) 35 , 36 for dense melts with arbitrary constitutive equations, which they solve using a pseudo-spectral method.

In the present work, we propose a new hybrid
approach to implementing hydrodynamic interactions
in dynamic SCF simulations. Starting from a minimal
model of coupled dynamic SCF and Navier-Stokes
equations, we propose a hybrid method to simulate
them efficiently. The dynamic SCF equations are
solved by a finite difference scheme,14, 37 , 38_{ which }

reduces the spurious current generation. The continuity equation and the Navier-Stokes equations are solved by the multiple-relaxation-time lattice Boltzmann method,39,40,41 which reduces the danger of numerical instabilities. The method can be applied both to polymer melts and solutions. Here we demonstrate its potential by studying two different types of systems. As a first test case, we investigate the kinetics of microphase separation in block copolymer melts. Then, we study the influence of hydrodynamics on vesicle formation in solutions of amphiphilic block copolymers.

This second application is motivated by the high
current interest in vesicle nanostructures. Vesicles
are closed membranes with usually spherical
topology. They are biologically important as model
systems for plasma membranes and sub-cellular
compartments in the living cells. Because of the
analogy to the natural systems and the compositional
simplicity, vesicles also serve as ideal platform for
understanding cellular membrane remodelling
processes such as fusion and fission of cells.42,43,44,45
Apart from their vital importance in biology, vesicles
also have extraordinary potential applications in
nanotechnology and biotechnology,46 , 47 , 48 , 49 _{for }

Although extensive experimental and theoretical
studies have been carried out in order to understand
the self-assembly of amphiphilic molecules into
vesicles and the remodelling of vesicles,50,51, much
less is known about the kinetics of vesicle formation
and vesicle remodeling under non-equilibrium
conditions. The mechanisms for such processes are
still subject to speculation.52 Computer simulations
provide a valuable alternative tool for studying such
systems at the microscopic and mescoscopic
levels.53 , 54 , 55 Various coarse-grained particle-based
molecular simulation approaches have been applied
to investigate evolution and remodeling processes of
vesicles.56,57,58,59,60,61,62,63,64 Among these, those using
implicit solvent models are particularly efficient, but
incorporating hydrodynamics is difficult. On the
other hand, most studies based on models with
explicit solvent were aimed at detailed simulations of
phenomena on small time and length scales, or
focussed on flat bilayers to study specific aspects of
membrane remodelling, due to the high
computational costs of simulating such fully explicit
models. Field-theoretical methods provide a
promising alternative approach to simulating systems
with larger volume over a longer time period. A
number of recent SCF and dynamic SCF studies have
therefore been devoted to studying membrane
dynamics and fusion, and vesicle formation and
fusion.65,66 ,67,68 ,69,70 ,71,72 Sevink and Zvelindovsky
used dynamic SCF simulations to investigate the
self-assembly behavior of block copolymer droplets
in solution with two hydrophobic blocks of different
hydrophobic strength.67,68_{ He and Schmid adopted a }

dynamic SCF method to examine the spontaneous vesicle formation in dilute solution of amphiphilic block copolymers.69,70,71.. Spherical and cylindrical micelles, toroidal and net-cage micelles as well as vesicles could be observed by tailoring the concentration and the hydrophilicity of the individual blocks. Moreover, a new pathway of vesicle formation was identified. These results are encouraging. However, hydrodynamic interactions, which should play an important role in solution, were neglected. Thus the effects of hydrodynamic flows on vesicle formation and vesicle remodeling are still not clear. This motivates us to reconsider the problem using our new hybrid simulation scheme.

The remainder of the paper is organized as follows: In the next section, we present the model equations and the hybrid simulation method. Then we discuss two applications in section 3. We first apply the

method to studying symmetric and asymmetric block copolymer melts (section 3.1). We recover the previous results cited above and analyze the role of bulk and shear viscosity. Then, we turn to studying vesicle formation in solution (section 3.2). The hydrodynamic flows are found to accelerate the vesicle formation and vesicle fusion in the amphiphilic block copolymer/solvent system significantly. The intermediate processes of vesicle formation and vesicle fusion are presented in detail. We summarize and conclude in section 4.

**2. MODEL EQUATIONS AND HYBRID **
**SIMULATION METHOD **

We consider a system with volume V, containing
*np *block copolymers (**AB**) and ns solvent beads (**S**).

(In copolymer melts, we simply set n*s* to zero.) All
copolymer molecules are represented by Gaussian
chains **A***n***B***m, consisting of Np=n+m beads with *
relative A fraction f=n/N*p* and statistical segment
length *a. The solvent consists of single “beads” *
(N*s*=1), each representing a collective of solvent
molecules. The volume and mass of beads are
denoted by *υ*I and mI, respectively, for beads of type

*I=A,B, or S. *

In our SCF theory, the free energy functional of the amphiphilic block copolymer/solvent system is defined as follows26,73

### { }

### ( ) ( )

### (

### )

### ( ) ( )

,

2 ln

! ! 1

2

1 2

*p* *s*
*n* *n*
*p* *s*

*I* *B* *I* *I*

*I*
*p* *s*

*IJ* *I* *J*

*I J*
*H*

*I* *I*
*I*

*F* *k T* *d* *U*

*n n*
*d d*

*d*

ρ ρ

ε ρ ρ

κ _{υ ρ}

Φ Φ

= − −

⎡ ⎤

⎣ ⎦

′ ′ ′

+ −

⎛ ⎞

+ _{⎜} − _{⎟}

⎝ ⎠

### ∑∫

### ∑∫

### ∑

### ∫

**r** **r** **r**

**r r** **r r** **r** **r**

**r**

** (1)**

Here, *kB* is the Boltzmann’s constant, T is the
temperature, the subscripts I and J∈*{A, B, S} are *
component indices, Φ*P is the intramolecular partition *
function for ideal Gaussian copolymer chains in the
external fields UA and UB, Φ*S is the partition function *
of solvent beads subject to the external field US, and
ρ*A*, ρ*B*, and ρ*S* are the local number densities of A, B,
and S beads, respectively. The third term on the right
hand side of Eq. (1) is the contribution from the
non-ideal mean-field interactions. It is characterized by
the energetic interaction *εIJ(|***r**-**r**′|) between beads I

and *J at positions ***r** and **r**′, which has the kernel

### ( )

### ( ) ( )

22 2

3

2 _{2}

3 2

3

0 _{exp}

*a*
*r*
*a*

*IJ*

*IJ* *r* =ε _{π} −

ε with constant cohesive

interaction parameter 0
*IJ*

constant local density by means of the Helfand
compressibility parameter *κH. The potentials UI are *
conjugated to the local density fields ρ*I* and must be
determined self-consistently from the relation

### { } ( )

### (

### )

### ( )

1 1 ' 1 ' d d 1 exp*N p* *P*

*p*

*n*
*p*

*A* *I* _{V}*N* *S*

*s*
*p*
*N*
*G*
*I* *s*
*s*
*B* *s*
*n*
*U*
*H* *U*
*k T*
ρ δ
=
′=
= −
⎡ ⎤

⎣ ⎦ _{Φ}

⎛ ⎛ ⎞⎞
× ⎜_{⎜}− ⎜_{⎜} + ⎟_{⎟}⎟_{⎟}
⎝ ⎠
⎝ ⎠

### ∑∫

### ∑

**r** **R** **R** **r R**

**R**
"

### { } ( )

### (

### )

### ( )

1 1 ' 1 ' d d 1 exp*p*

*Np*

*P*

*p*

*N*

*p*

*B* *I* _{V}*N* *S*

*s n*
*p*
*N*
*G*
*I* *s*
*s*
*B* *s*
*n*
*U*
*H* *U*
*k T*
ρ δ
= +
′=
= −
⎡ ⎤

⎣ ⎦ _{Φ}

⎛ ⎛ ⎞⎞
× ⎜_{⎜}− ⎜_{⎜} + ⎟_{⎟}⎟_{⎟}
⎝ ⎠
⎝ ⎠

### ∑ ∫

### ∑

**r** **R** **R** **r R**

**R**

"

(**2**)

### { } ( )

*s*exp 1

### ( )

*S* *I* *S*

*s* *B*

*n*

*U* *U*

*k T*

ρ ⎡_{⎣} ⎤_{⎦} = ⎛_{⎜}− ⎞_{⎟}

Φ _{⎝} _{⎠}

**r** **r**

where **R***s is the position of bead s and Is its type (A *

or B). The Edwards Hamiltonian for the Gaussian
chain is given by = *B*

### ∑

*N*

_{=}

*P*

### (

−_{−}

### )

*s* *s* *s*

*a*
*T*
*k*
*G*

*H* _{2} 2

1 2

3

2 **R** **R** .

To account for hydrodynamic flows, the time
evolution of the density fields ρ*I*(**r**) is described by
convection-diffusion equations with local kinetic
coupling coefficient

### ( )

_{(}

_{( ) ( )}

_{)}

### ( )

### ( )

### ( )

, , , , , ,*I*

*I*

*I* *I* *I* *I*

*t*

*t* *t*

*t*

*M* *t* *t* *t*

ρ

ρ

ρ μ ξ

∂

+ ∇ ⋅ ∂

= ∇ ⋅ ∇ +

**r**

**r** **u r**

**r** **r** **r**

** (3)**

Here, μ* _{I}* =δ

*F*δρ

*is the intrinsic chemical potential,*

_{I}### (

### ) ( )

### (

### )

d d ' | ' | ' 1

*I* *I* *IJ* *J*

*J*

*H I* *J* *J* *J*

*U*

μ ε ρ

κ υ υ ρ

= − + −

+ −

### ∑∫

### ∑

**r r** **r r** **r**

** (4)**

*MI is the mobility coefficient of beads of type I, and *

*ξI * is a stochastic noise satisfying the
fluctuation-dissipation relation

### ( )

,*t*=0

*I* **r**
ξ **,**

### ( ) ( )

### ( ) (

### ) (

### )

, , 2 ,*I*

*J*

*B* *IJ* *I* *I*

*t* *t*

*k T M* *t* *t t*

ξ ξ

δ ρ δ δ

′ ′

′ ′

= − ∇⋅ ∇ − −

**r** **r**

**r** **r r**

** (5)**

The velocity field **u** of fluid obeys the continuity

equation and the fluctuating Navier-Stokes equations, which read

### ( )

ρ*u*α β

### (

ρ*u*α

*u*β

### )

βσαβ βσαβ*f*α β

*P*αβ

*t* +∂ =∂ +∂ ′ + −∂

∂ **. (6)**

Here _{I}_{I}

*Im*

ρ=

### ∑

ρ is the total local mass density of the fluid, σ_{αβ}and σ

_{αβ}′ are deterministic and stochastic

stress tensors, and the last two terms, (*f*_{α} − ∂_{β αβ}*P* ),
summarize the local volume forces acting on the
fluid. The deterministic stress tensor σ_{αβ} is linearly
proportional to the velocity gradient, σ_{αβ}=η_{αβγδ}∂_{γ}*u*_{δ}
with η_{αβγδ}=η_{s}

### (

δ_{αγ}δ

_{βδ}+δ

_{αδ}δ

_{βγ}

### )

+### (

η*−*

_{b}_{3}2η

_{s}### )

δ_{αβ}δ

_{γδ}

_{, where }η

_{s is }the shear viscosity and η*b* the bulk viscosity. The
fluctuating stress σ_{αβ}′ is related to the viscosity by
means of the fluctuation-dissipation theorem

### ( )

### ( ) ( )

### (

### ) (

### )

, 0,

, , 2 _{B}

*t*

*t* *t* *k T* *t t*

αβ

αβ γδ αβγδ

σ

σ σ η δ δ

′ =

′ ′ ′ ′ = − ′ − ′

**r**

**r** **r** **r r**

**.(7)**

Finally, the local volume forces, (*f*_{α} − ∂_{β αβ}*P* ), may
result from a pressure gradient or from external fields.
In a one-component fluid with small density
variations, the pressure tensor can be approximated
by _{const.+} 2

*s*

*P*_{αβ} = δ_{αβ}*c* ρ, where csis the isothermal
speed of sound. We note that the constant does not
contribute to Eq. (6) and can thus be omitted. In our
multicomponent system, the coupling of the
Navier-Stokes equations with the free energy density
functional (1) can be implemented either by
introducing an additional contribution to the pressure
term, or a thermodynamic volume force fα . These
two approaches are equivalent. Here we choose the
force approach, i.e., we introduce the volume force32

### ( )

=−_{∑}

### ( )

∇### ( )

*I*

*I*

*I* *t* *t*

*t* , ,

, **r** **r**

**r**

**f** ρ μ ** ** ** (8) **

This completes the definition of the basic model which must now be solved numerically. In the following, we propose a hybrid algorithm that solves the fluid dynamics part (Eq. (5)) via a multiple-relaxation-time lattice Boltzmann (LB) method and the density functional part (Eq. (3)) via a finite difference scheme.

In the LB method, the space is discretized by a
lattice, and each lattice site** r** carries a set of discrete

velocity distribution functions ni(**r**,t), which describe

the partial density of fluid particles with velocity **c***i at *

time *t. The total density ρ*(**r**,t) and momentum

density** j**(**r**,t) are related to the moments of the

distribution functions74

### ( )

=_{∑}

### ( )

*i*

*i*

*t*

*n*

*t*, ,

**r**

**r**ρ

**,**

### ( )

### ( ) ( )

### ( )

12

, , , * _{i}* ,

_{i}*i*

*t* =ρ *t* *t* =

### ∑

*n*

*t*+ Δ

*t*

The sum runs over the discrete velocity space {**c***i}. In *

the following, we adopt the popular D3Q19 model, 75
which is based on a cubic lattice and whose velocity
set contains the zero velocity and the vectors that
connect each node with its nearest and next-nearest
neighbors. Here the velocity unit is the “lattice
velocity” c=h/Δ*t with the lattice parameter h and the *
time step Δ*t. *

Within one time step Δ*t, the distribution *
functions ni evolve according to

### (

### )

### ( )

### ( )

### ( )

*

, ,

: , ,

*i* *i* *i*

*f*

*i* *i* *i* *i*

*n* *t t* *t* *n* *t*

*n* *t* *t*

+ Δ + Δ =

′
= + Δ ⎡_{⎣} ⎤_{⎦}+ Δ + Δ

**r c** **r**

**r** **n r**

** ** ** (10)**

i.e., the distributions are first reshuffled from n*i* to n*i**
(collision step) and then shifted to neighboring sites
according to their respective velocities (streaming
step). The collision step mimics particle scattering
events in the fluid (Δ ⎡_{i}_{⎣}**n r**

### ( )

,*t*⎤

_{⎦}) as well as the effects of the volume forces (Δ

*if*) and stress fluctuations (Δ

*i*′). Specifically, the scattering contribution relaxes the distributions nj towards the equilibrium distributions

*eq*
*j*

*n* with a linear collision operator L*ij *to be specified

below,

### ( )

,### (

*eq*

### )

*i* *t* *L nij* *j* *nj*

Δ ⎡_{⎣}**n r** ⎤_{⎦}= − . In the D3Q19
model, the equilibrium distribution for given density
ρ and fluid velocity **u** is given by

### ( )

2 4 221 1
, 1
2 2
*i* *i*
*eq* *i*
*i* *i*

*s* *s* *s*

*u u c c*

*u c* *u*

*n*

*c* *c* *c*

α β α β α α

ρ =ρ ω ⎛_{⎜} + + − ⎞_{⎟}

⎝ ⎠

**u** **, (11)**

where *c _{s}* =

*c*3 is the isothermal speed of sound, and the weight coefficients are

*ω*0=1/3,

*ω*1-6=1/18,

and *ω*7-18=1/36. It is constructed as an expansion in

the velocity up to second order that satisfies the
constraints *eq*

*i*

*in* =ρ

### ∑

,*eq*

*i* *i*

*in c*α =ρ*u*α

### ∑

, and*eq*
*i* *i* *i*

*in c c*α β =ρ*u u*α β +*P*αβ

### ∑

with 2*s*

*P*_{αβ} =δ_{αβ} *c* ρ.
The simplest choice of the collision operator18 is
*Lij=-*δ*ij/*τ*, *corresponding to a single relaxation time
that determines both the bulk and shear viscosity. In
this paper, we employ a more sophisticated scheme,
the multiple-relaxation-time model39,40,41, which has
the advantage that the mass and momentum are
conserved rigorously and that both viscosities can be
varied independently. The scheme has recently been
reviewed in detail by Dünweg and coworkers19,76 and
we will refer the reader to these references for details
and derivations. Basically, one constructs
eigenvectors **e**k of the collision operator Lij from

outer products of the velocities **c**i, which are mutually

orthogonal with respect to the scalar product

*i* *ki kl*
*i*ω *e e*

### ∑

and relaxes them individually with relaxation parameters γ*k, corresponding to relaxation*rates (1−γ

*) /Δ*

_{k}*t*. The first four eigenvectors,

**e**0-

**e**3,

correspond to the conserved modes (mass and momentum) and have the relaxation parameter γ0-3=1.

In choosing the higher eigenvectors, one has some freedom. The D3Q19 eigenvectors and relaxation parameters used in the present work are summarized in Table 1.

**Table 1 **Basis set of the D3Q19 model

**e***ki* denotes eigenvector and γ*k* the relaxation parameter.

*k* **e***ki * γ*k* *k * **e***ki * γ*k*

0 1 1 10

### (

_{3}2

_{5}

*2*

_{c}### )

_{c}*3*

_{c}*ix*
*i* −

**c** 0

1 *c _{ix}*

*c*1 11

### (

_{3}2

_{5}

*2*

_{c}### )

_{c}*3*

_{c}*iy*

*i*−

**c** 0

2 _{c}_{iy}* _{c}* 1 12

### (

_{3}2

_{5}

*2*

_{c}### )

_{c}*3*

_{c}*iz*

*i*−

**c** 0

3 *c _{iz}*

*c*1 13

### (

*2*

_{c}*2*

_{c}### )

_{c}*3*

_{c}*ix*

*iz*

*iy*− 0

4 2 * _{c}*2

_{−}

_{1}

*i*

**c** γ*b* 14

### (

*ciz*2 −

*cix*2

### )

*ciy*

*c*3 0

5

### (

*2*

_{c}*2*

_{c}### )

*2*

_{c}*iy*

*ix* − γ*s* 15

### (

### )

3 2

2 _{c}_{c}_{c}

*c _{ix}*−

_{iy}*0 6*

_{iz}### (

2_{3}

*2*

_{c}### )

*2*

_{c}*iz*
*i* −

**c** γ*s* 16 3**c*** _{i}*4

*c*4 −6

**c**

*2*

_{i}*c*2 +1 0

7 _{c}_{c}* _{c}*2

*iy*

*ix* γ*s* 17

### (

### )(

### )

4 2 2 2

2 _{3}

2**c*** _{i}* −

*c*

*c*−

_{ix}*c*

_{iy}*c*0 8

_{c}

_{c}*2*

_{c}*iz*

*ix* γ*s* 18

### (

### )(

### )

4 2 2 2

2 _{3} _{3}

2**c***i* − *c* **c***i* − *ciz* *c* 0
9 _{c}_{c}* _{c}*2

*iz*

*iy* γ*s*

The nonequilibrium distribution ( *eq*)

*i* *i*

*n* −*n* and
the forcing terms *f*

*i*

Δ are then expanded in moments using the basis vectors eki19,76

( *eq*)

*k* _{i}*i* *i* *ki*

*m* =

### ∑

*n*−

*n*

*e*

**,**

*m*=

_{k}f### ∑

*Δ*

_{i}*f*

_{i}e_{ki}**, (12)**

which evolve during the collision step according to

*k*
*k*
*f*
*k*
*k*
*k*

*k* *m* *m* *r*

*m** =γ + +ϕ

**. ** ** (13) **

Here _{k}_{Tb}

### (

_{1}2

### ) ( )

*2*

_{c}*3*

_{h}*s*

*k*

*k*

*B*

*k* ρ γ

ϕ = − is the amplitude of

the random noise for the k-th mode with

### ∑

= _{i}*i* *ki*

*k* *e*

*b* _{ω} 2 _{, and r}

*k* is a Gaussian random number
with zero mean and unit variance. Exploiting the
orthogonality of the eigenvectors, one can easily
reconstruct the new distribution function after

collision, * *eq* 1

*i* *i* *i* *k* *k* *k* *ki*

*n* _{=} *n* _{+}ω

### ∑

*b m e*− ∗

_{. Finally, the }

collision operators of the forcing terms are given by19

### (

### )

⎥ ⎦ ⎤ ⎢ ⎣ ⎡ − + Δ =Δ ω _{α} _{α} _{αβ} _{α} _{β} 2δ_{αβ}

2
2 _{2}
1
*s*
*i*
*i*
*s*
*i*
*s*
*i*
*f*

*i* *Σ* *c* *c* *c*

with

### (

### )

### (

α β β α γ γ αβ### )

### (

### )

γ γ αβαβ γ *u* *f* *u* *f* *u* *f*δ γ *u* *f*δ

*Σ* = + * _{s}* + − + 1+

_{b}3
1
1
2
1
3
2 _{. }

The multiple-time relaxation LB model described above solves Eq. (5) for a pressure term of the form

2

const.+ _{s}

*P*_{αβ} = δ_{αβ}*c* ρ* and arbitrary volume forces ***f**.

The shear viscosity η*s and bulk viscosity *η*b* are
related to *γs* and *γb*, respectively, via76

2
1
2 1
*s* *s*
*s*
*s*

*t c*ρ γ
η
γ
Δ +
=
− **, **
2
1
3 1
*s* *b*
*b*
*b*

*t c*ρ γ
η

γ

Δ +

=

− ** (15)**

The remaining equations, the set of
convection-diffusion equations (3), are integrated numerically
via a finite-difference scheme on the same lattice
nodes used for the lattice Boltzmann method. The
diffusion part of the equations has been implemented
by the implicit Crank-Nicholson algorithm77 and the
convection term of the equations is discretized using
the explicit two-step Lax-Wendroff scheme.78 The
thermal noise terms *ξI(***r**,t) are calculated by an

algorithm due to Vlimmeren and Fraaije.79_{ The }

Gaussian chain density functional of I-type bead is expressed in terms of Green’s propagators

### ( )

### ( )

1### ( )

1
*n*

*A* *s* *s*

*s*

*G* *G*

ρ σ +

+ =

⎡ ⎤

∝

### ∑

_{⎣}

_{⎦}

**r** **r** **r** **, **

### ( )

### ( )

1### ( )

1

*P*

*N*

*B* *i* *s*

*s n*

*G* *G*

ρ σ +

+ = +

⎡ ⎤

∝

### ∑

_{⎣}

_{⎦}

**r** **r** **r** **, ** ** (16)**

where the set of integrated Green’s functions Gsand
inverse Green’s functions *G _{s}*+ are related by
recurrence relations

### ( )

exp*s*

### ( )

### [

1### ]

### ( )

*I*

*s* *s*

*B*

*U*

*G* *G*

*k T* σ −

⎛ ⎞

= ⎜_{⎜}− ⎟_{⎟}

⎝ ⎠

**r**

**r** **r** **, **

### ( )

exp*s*

### ( )

1### ( )

*I*

*s* *s*

*B*

*U*

*G* *G*

*k T* σ

+ +
+
⎛ ⎞
⎡ ⎤
= ⎜_{⎜}− ⎟_{⎟} _{⎣} _{⎦}
⎝ ⎠
**r**

**r** **r** ** (17)**

subject to the initial conditions 0

### ( )

= 1### ( )

=1+
+ **r**
**r**
*P*
*N*
*G*
*G* ,

and the linkage operator *σ* denotes convolution with
the Gaussian kernel

### [ ]

### ( )

## (

2### (

### )

## )

### ( )

2 3 2 3 2 2 3 exp

2 *V* *a*

*f* *d* *f*

*a*
σ
π
⎛ ⎞ _{′} _{′} _{′}
=_{⎜} _{⎟} − −
⎝ ⎠

### ∫

**r** **r** **r r** **r** .

This completes the description of our hybrid LB/SCF simulation method. In our simulations, we chose the time steps to be identical for the LB and the dynamic SCF simulations, i.e. LB steps alternate with propagations of the convection-diffusion equation (3). Multiple time step schemes are also conceivable, but have not been explored here. We

note that every propagation step of Eq. (3) involves the self-consistent determination of the potentials UI

(see Eq. (4)) from Eqs. (16) and (17). This was done with the Fletcher-Reeves nonlinear conjugate gradient method. The Gaussian integrals (17) were integrated with a 27-point stencil scheme26.

In the following section, we will describe a number
of applications to copolymer systems. The bead
volume, the bead mass, and the mobility coefficient
in these studies are taken to be equal for all bead
species, i.e., υ*A=*υ*B=*υ*S *=:υ0, mA=mB=mS=:m0, and

*MA=MB=MS =:M. The basic length unit is the lattice *
parameter *h, the basic energy unit is the thermal *
energy kBT, and the basic time unit is 2

*B*

*h k T M*

τ = .

In the remaining paper, all quantities shall be given
in these units. For example, the basic viscosity unit is
η***_{=k}

*BT*τ/h3.

An important parameter of the simulation is the
time step Δ*t, which sets the lattice velocity c=h/*Δ*t *
and hence the speed of sound c*s*in the model. In a
typical simulation setup, csis much smaller than the
real speed of sound. This is not a problem since we
are interested in slow diffusive processes and c*s* is
not a physically relevant parameter in our context.
However, we must carefully ensure that our
processes are indeed slow compared to the value of
*cs* in our model.

The other model parameters are the statistical
segment length, which we set to a=1.1543 h for
practical reasons80, the “bead” mass m*0*, which we set
to m0= 1 kBTτ*2*/h2, the “bead” volume υ0, which sets

the noise scaling parameter81Ω=h3/υ0, the Helfand

compressibility parameter k*H* , which we set to
*kH*υ0/kBT= 10, the Flory-Huggins parameters

### (

### )

### (

0### )

0 0 0

0 _{2}_{ε} _{ε} _{ε} _{2} _{υ}

χ* _{IJ}* =

*−*

_{IJ}*−*

_{II}

_{JJ}*k*, and the bulk and shear viscosity η

_{B}T*s and*η

*b, which are related to the*relaxation parameters

*γs and γb via Eq. (15).*

Unless stated otherwise (i.e., for all simulations
except those belonging to Figure 2), we have chosen
the noise parameter Ω=400 and our simulations were
carried out in boxes of size 64h×64h×64h with period
boundary conditions, using a time step of Δ*t/*τ=0.4.
For every system and every choice of parameter set,
we have carried out five independent runs with
different random seeds.

We can get a rough idea about the values of our
simulation units in terms of SI units by matching the
temperature T=300K, the radius of gyration of the
polymers Rg, and their cooperative diffusion constant
*DP*. In the simulations, we have *Rg* =*a* *N*/6 and

*TN*
*k*
*M*

chains of length N~10 beads. Mapping real chains of
size *Rg~3nm, we conclude that our length unit *
corresponds to h~2nm. The diffusion constant of
polymers is of order Dp~10-6cm2/s in solution, and
*Dp*~10-9cm2/s in dense melts. Mapping this to the
simulations yields the time units τ~4⋅10-9s in solution,
and τ~4⋅10-6s in dense melts. The corresponding
basic viscosity unit is η*~2⋅10-3Ns/m2 in solution,
which is of the order of the shear viscosity of water
(η~0.8⋅10-3_{Ns/m}2 _{), and }_{η}_{*~2}_{⋅}_{Ns/m}2 _{in dense melts. }

**3.RESULTS **

**3.1 Dynamics of Microphase Separation in Block **
**Copolymer Melts **

We first use our method to investigate the effect of hydrodynamics on the kinetics of microphase separation in block copolymer melts. To this end, we have quenched systems of symmetric A8B8 block

copolymers (Gaussian chains, f=0.5) from an
initially disordered state into an ordered state with
Flory-Huggins interaction parameter 0 _{1.0}

*AB*

χ = . This
parameter has been chosen such that lamellar
structures are generated according to the phase
diagrams obtained by the static self-consistent field
calculation.82. The initial configurations were thus
homogeneous density distributions. In order to
compare the results of our model with those of a
system without hydrodynamic flows, we also
performed simulations based on the diffusion-only
model, which is defined by Eq. (3) with **u**=0.

Figure 1 shows the time evolution of three characteristic quantities during the microphase separation under different hydrodynamic conditions. The top panel displays the evolution with time of the free energy density and an order parameter defined

as =

### ∫ ∑

### (

−### )

*V* *I* *I* *I*

*V*

*t*

*S*_{(} _{)} 1 φ φ0 2 _{, where}
*I*

φ =ρ*I*υ0 and φ*I*0

are, respectively, the local and average volume fractions of I-type beads in the system. The lower panel shows two series of corresponding simulation snapshots, one for a purely diffusive system and one for a system with hydrodynamics (convection-diffusion model).

At the beginning, hydrodynamic flows are found to have little effect on the phase separation process (insets of Figure 1, snapshots at t=200τ). A sharp increase of the order parameter in the initial stage of the simulation, accompanied by a rapid decrease of the free energy, indicates that the microphase

separation sets in within 20τ after the quench, and the curves for systems with and without hydrodynamics lie on top of each other. The simulation snapshots at times 200τ illustrate that the patterns are still very similar. At this initial stage, hydrodynamic effects can thus be neglected.

**0** **10000** **20000** **30000** **40000**
**0.238**

**0.240**
**0.242**
**0.244**
**0.246**

**0** **100** **200**
**0.245**

**0.250** **diffusion only**

η

**s/**η

∗

**=0.36**

η

**s/**η

∗

**=0.22**

υ**0**

**F/**

**(k****B**

**TV**

**)**

**Time/**τ

**0** **10000** **20000** **30000** **40000**

**0.35**
**0.40**
**0.45**

**0** **100** **200**
**0.2**

**0.3**

**0.4** _{diffusion only}

η**s/**η

∗
**=0.36**

η** _{s}/**η∗

**=0.22**

**S**

**Time/**τ

**t****=200****τ**** ****t****=2000****τ**** ****t****=6000****τ**** ****t****=40000****τ**

**Figure 1** Top panel: Time evolution of the free energy density

### (

*k*

*TV*

### )

*F* *B*
0

υ and the segregation parameter *S* during the

microphase separation process of A8B8 block copolymers after a

quench from the disordered state, with and without hydrodynamics for various values of shear viscosity at fixed

bulk viscosity η*b=*0.34η*. The insets show blowup for early

times. Error bars are omitted for clarity. Middle and bottom panel: Corresponding configuration snapshots without

hydrodynamics (middle) and with hydrodynamics (bottom*, *

η*s=*0.22η*and η*b=*0.34η*) at times as indicated. Red regions

indicate A-rich regions, green surfaces show isodensity surfaces

*A*

**0** **3000** **6000** **9000** **12000**
**0.242**

**0.244**
**0.246**
**0.248**

**0** **50** **100**

**0.250**
**0.255**

**(a1)**

**diffusion only **

η** _{s}/**η∗

**=1.55**

η** _{s}/**η∗

**=0.28**

υ**0**

**F/**

**(k****B**

**TV**

**)**

**Time/**τ

**0** **3000** **6000** **9000** **12000**

**0.269**
**0.270**
**0.271**
**0.272**
**0.273**

**(b1)**

**diffusion only **

η** _{s}/**η∗

**=1.55**

η** _{s}/**η∗

**=0.28**

υ**0**

**F/**

**(k****B**

**TV**

**)**

**Time/**τ

**0** **3000** **6000** **9000** **12000**

**0.242**
**0.244**
**0.246**
**0.248**

**(a2)**

**diffusion only **

η
**b/**η

∗
**=1.03**

η** _{b}/**η∗

**=0.18**

υ**0**

**F/**

**(k****B**

**TV**

**)**

**Time/**τ

**0** **3000** **6000** **9000** **12000**

**0.269**
**0.270**
**0.271**
**0.272**
**0.273**

**(b2)**

**diffusion only **

η** _{b}/**η∗

**=1.03**

η** _{b}/**η∗

**=0.18**

υ**0**

**F/**

**(k****B**

**TV**

**)**

**Time/**τ

**Figure 2** Microphase separation in a system of (a) symmetric (A8B8) and (b) asymmetric (A5B11) block copolymers upon quenching

into the ordered phase from an initially disordered solution, without and with hydrodynamics. Top: Final configuration after 12000 τ

without and with hydrodynamics (color coding as in Figure 1). Bottom: Evolution of free energy (a1, b1) for various values of shear

viscosity η*s* at fixed bulk viscosity η*b=*0.56η*; (a2, b2) various values of η*b* at fixed η*s=*0.83η***. Error bars are omitted for clarity.

Inset in (a1) shows blowup in the initial stage. In all simulations, the noise parameter for the convection-diffusion dynamics was set to

Ω=100 and the hydrodynamic noise was turned off.

Shortly after that, however, the hydrodynamic flows
begin to have a pronounced effect on the time
evolution. In the presence of hydrodynamic
interactions, the system orders faster, the free energy
drops faster, and the ordered domains grow faster.
Both the diffusive system and the systems with
hydrodynamics tend to get trapped in metastable
states directly after the quench. This leads to the
formation of a plateau in the free energy curve at
early times, t~1000τ. In the presence of
hydrodynamics, the systems manage to escape this
metastable plateau within the time t~10000τ*. Purely *
diffusive systems remain trapped and order only very

slowly. Even though they show local lamellar order at the end of the simulation runs (40000τ), the configurations are still filled with defects. The mean free energy is still higher than that of systems with hydrodynamic interactions. Thus the main effect of convective flows on the evolution process of the microstructures is to promote the removal of defects. The lower the shear viscosity, the more effective they are. We conclude that hydrodynamic interactions help the system to overcome free energy barriers and to access its final equilibrium ordered state.

Next we have studied the influence of different model parameters on this effect, i.e., we have varied

With hydrodynamics

η*s=*0.28η**,*η*b=*0.56η

no hydrodynamics diffusion only with hydrodynamics

η*s=*0.28η**,*η*b=*0.56η*

no hydrodynamics (diffusion only

the bulk and shear viscosity separately, and we have also considered asymmetric copolymers that order into a different morphology. To assess the influence of the noise, we have also chosen a different noise scaling parameter, Ω=100, and turned off the noise in the LB part of the simulations (i.e., ϕk=0 in Eq. (13),

which corresponds to setting σ_{αβ}′ =0 in Eq. (6)).
These studies were carried out in smaller systems of
size 48h×48h×48h.and a time step Δ*t/*τ=0.2. The
results are summarized in Figure 2.

Figure 2(a) shows the evolution of systems of symmetric A8B8 block copolymers after quenching

from the disordered phase into the lamellar phase at

0 _{1.0}

*AB*

χ = for various combinations of shear and bulk
viscosity. In Figure 2 (a1), the bulk viscosity η*b* is
kept constant and the shear viscosity η*s is varied, *
which corresponds to the situation studied in Figure
1. The results are very similar. Hydrodynamic flows
accelerate the ordering and help to remove lamellar
defects. The ordering in the diffusive case is faster
than in the systems of Figure 1, which can
presumably be attributed to the smaller system size
and/or the higher noise level. In the presence of the
long-range hydrodynamic interactions, the ordering
time becomes comparable. Furthermore, the free
energy density of the equilibrated final state is higher
than in Figure°1. This is also an effect of the higher
noise level (the amplitude of the noise is inversely
proportional to Ω) and the ensuing slightly weaker
segregation of the components. Indeed, the order
parameter in the system of Figure 2(a) tends to
S→0.425 at large times (data not shown) as opposed
to S →0.46 in Figure°1. Apart from this slight effect
on the final equilibrium state, the noise has no
qualitative influence on the results. Hydrodynamic
interactions are still found to accelerate the ordering
during the whole process of microphase separation,
until equilibrium is reached.

This is different for asymmetric block copolymers. Figure 2(b) shows the time evolution of the free energy density during the microphase separation of A5B11 block copolymers (f=0.31) for

the cases of the diffusion-only model and different
realizations of the convection-diffusion model. The
systems were quenched from an initially disordered
state 0 _{0}

*AB*

χ = to an ordered state at 0 _{1.3}
*AB*

χ = . Under these conditions, the asymmetric block copolymers should self-assemble into a hexagonal array of cylindrical microstructures according to the mean-field theory.82 Initially, the behaviour of the free energy density is similar to that of symmetric block

copolymers. It decreases more rapidly in the presence of convective flows than in purely diffusive systems. The hydrodynamic interactions promote the ordering process at early times. Once the system is locally ordered, however, they are no longer effective, and the system remains trapped in metastable states just like in the diffusive case. The final snapshots after the total run length of 12000τ feature a disordered mess of entangled cylindrical microstructures, which looks very much alike for the diffusive and the convective-diffusive system. In contrast, the convective flows in systems of symmetric block copolymers help to remove the defects of microstructures not only in the early stage, but also at intermediate and late stages of the microphase separation.

Inspecting in more detail the influence of the
different viscosity parameters, we finds that the key
quantity is clearly the shear viscosity η*s. Varying the *
bulk viscosity η*b* at fixed shear viscosity has only a
small effect on the time evolution (Figure 2 a2 and
b2). By varying the shear viscosity η*s, on the other *
hand, one can influence the ordering process
significantly (Figure 1 and Figure 2, a1 and b1). The
hydrodynamic interactions are most effective at small
shear viscosity η*s. *

a minor role. Thus our method applied to block copolymers gives reasonable results compared to earlier work based on different methods as well as to theoretical expectations. This encourages us to apply it to a more complex system in the next step.

**3.2Kinetics of Vesicle Formation of Amphiphilic **
**Block Copolymers in Solution **

As a second application example, we study the kinetics of nanostructure self-assembly in copolymer solutions. The model block copolymers are represented by A2B8 Gaussian chains in a solvent S.

The Flory-Huggins interaction parameters are set
to 0 _{2.3}

*AB*

χ = , 0 _{2.4}

*BS*

χ = , and 0 _{0.25}

*AS*

χ = . Thus A

blocks and B blocks are incompatible, the A block is hydrophilic, and the B block is hydrophobic. The average volume fraction of amphiphilic block copolymers in solution is set to 0.2. These parameters are chosen in the spinodal region of the homogenous mean-field phase diagram83, i.e., the system will phase separate after quenching from the homogenous state69. Mapping the diffusion constant and the radius of gyration of the molecules to those of real copolymer systems71, we find that our length unit, h, is in the range of a few nm, and the time unit

*τ* corresponds to roughly 10-9_{s. }

In this work, we focus on the effect of hydrodynamic flows on the dynamics of spontaneous vesicle formation and vesicle fusion. Motivated by the previous finding in Section 3.1 that the bulk viscosity ηbis not a very influential parameter, we

fix η*b/*η**=0.34 * and vary the value of the shear
viscosity η*s* only. Like before, we have also
performed based on the diffusion-only model for
comparison.

Figure 3 compares the evolution with time of the free energy density and the degree of segregation,

characterized by the quantity

### ( )

### ( )

### ( )

### ( )

### ∫

+ − −=*V*1 *d***r** *A* **r** *B* **r** *A*0 **r** *B*0 **r**

*S* φ φ φ φ , during the

aggregation process in the absence and presence of hydrodynamic flows. Like in the copolymer melt, the effect of hydrodynamic interactions is small in the initial stage (inset). The convective flows have only a weak effect on the spinodal decomposition of the amphiphilic block copolymers. After an initial “incubation time” where spinodal fluctuations build up until they reach a critical threshold69, the free energy suddenly drops and the segregation parameter rises sharply, indicating that the amphiphilic block copolymers begin to aggregate into clusters. This is followed by a period of cluster growth and reorgani-

**0** **10000** **20000** **30000** **40000**

**0.00**
**0.01**
**0.02**
**0.03**
**0.04**

**diffusion only**

η** _{s}/**η∗

**=0.36**

η** _{s}/**η∗

**=0.22**

**0** **100** **200**

**0.03**
**0.06**

υ**0**

**F/**

**(k****B**

**TV**

**)**

**Time/**τ

**0** **10000** **20000** **30000** **40000**

**0.18**
**0.21**
**0.24**
**0.27**
**0.30**

**diffusion only**

η** _{s}/**η∗

**=0.36**

η** _{s}/**η∗

**=0.22**

**S**

**Time/**τ

**Figure 3** Time evolution of the free energy density

### (

*k*

*TV*

### )

*F* *B*
0

υ and the segregation parameter during the

quenching process of amphiphilic block copolymers in solution for simulations with and without hydrodynamics. The inset shows the free energy density as a function of time in the initial

stage. The bulk viscosity is η*b=*0.34η*, the shear viscosity η*s* is

varied as indicated in the graphs.

zation, which is accompanied by slower further segregation and free energy decrease. In these intermediate and late stages, hydrodynamic flows become important and significantly accelerate the self-organization process. Like in the case of copolymer melts, the hydrodynamic effects on the free energy are strongest for small shear viscosities.

**(a1) ****t****=200****τ**** ****(a2) ****t****=800****τ**** (a3) ****t****=3600**** ****(a4) ****t****=40000****τ**

**(b1) ****t****=200****τ**** ****(b2) ****t****=800****τ**** (b3) ****t****=3600****τ****(b4) ****t****=40000****τ****Figure 4** Pattern evolution during the self-assembly of
amphiphilic block copolymers (a) in the diffusion-only model

(top) and (b) with hydrodynamics (bottom, shear viscosity

η*s=*0.22η*, and bulk viscosity η*b=*0.34η*) at simulation times *t*

as indicated. Colour coding as in Fig.1. The arrow in (a3) points to a bilayer.

semivesicles which contain A-blocks in the center (snapshots a3 and b2). The semi-vesicles further coalesce with neighboring small spherical micelles, solvent diffuses into the inner parts of aggregates until, finally, vesicles are formed (snapshots a4 and b4). In the late stage of the process, vesicle fusion events are also observed, which is why some of the vesicles in Figures 4, a4 and b4 are elongated.

The self-assembly of vesicles from micelles via semi-vesicles is illustrated in more detail in Figure 5. Here, we start from an identical configuration containing several micelles, which has been generated by a diffusion-only simulation, and monitor its evolution in the presence and absence of hydrodynamic flows. The pathway of vesicle formation is similar in both cases. First, spherical micelles coalesce to form a cylindrical micelle (snapshots a2 and b2). The solvent content in the inner parts of the micelle is very small due to the hydrophobicity of the B-beads (Figure 5c). Then the short cylindrical micelle gradually retracts towards a spherical shape. Once the micelle diameter exceeds a certain size in the process of retraction, the amphiphilic block copolymers start to flip-flop and reorganize into a semi-vesicle (snapshots a3-a4, b3-b4). The solvent diffuses through the hydrophobic B-bead regions and swells the hydrophilic A-B-beads in the cores of aggregates. Thus the semi-vesicle contain some hydration solvent in the core part, but no interior bulk solvent (Figure 5d). The semi-vesicle further merges with neighbour micelles (snapshots a5 and b5). The joint aggregate retracts again into a spherical shape and solvent diffuses into the inner part of the aggregate to form the interior bulk solvent (snapshots a6 and b6). The final vesicle contains a

**(a1)**** t****=2600****τ**** ** ** (a3)**** t****=3800****τ**** ****(a5) ****t****=6800****τ**** **** (a2) ****t****=3400****τ**** ****(a4) ****t****=6400 (a6)**** t****=8000****τ**

**(b1)**** t****=2600****τ**** (b3) ****t****=2780****τ**** **** (b5) ****t****= 3160****τ**** (b2) ****t****=2640****τ**** ****(b4) ****t****=2840****τ**** **** (b6)**** t****=3300****τ**

** (c) (d) (e) **

**Figure 5** Simulation snapshots during the late stage of vesicle
formation in the (a) absence and (b) presence of hydrodynamic
effects. The snapshots are extracted from identical regions of a
much larger simulation box. The initial configuration at time

2600*τ* is the same in both cases and was generated from a

diffusion-only simulation. The convective flows were then

turned on at *t*=2600*τ* in the simulation corresponding to in panel

(b). In panels (a) and (b), the evolution time is shown below each snapshot. The shear viscosity and bulk viscosity are

η*s=*0.22η* and η*b=*0.34η*, respectively. Panels (c), (d), and (e)

show the volume fraction distributions of solvent beads in a cross section of the aggregates marked with arrows in the

panels (a2), (a4), and (a6) at time 3400*τ*, 6400*τ*, and 8000*τ*,

respectively.

significant amount of interior bulk solvent (Figure 5e).

Comparing the simulations with and without
hydrodynamic interactions, we find the pathways of
vesicle formation to be qualitatively very similar.
The sequence of structures, spherical micelle–
cylindrical micelle–semi-vesicle–vesicle, is the same.
However, the presence of hydrodynamic effects
remarkably accelerates the formation of vesicles. For
instance, at time 3300*τ*, the initial four spherical
micelles have completed the whole process of
evolution into a vesicle as the convective flows are
included in the simulation (Figure 5, b6), whereas
they have barely managed to merge into a short
cylindrical micelle in the diffusion-only model
(Figure 5, a2) and need another 4500*τ* to reach the
final vesicle state.

The pathway described above is the main mechanism of vesicle formation for the set of parameters chosen in this study. It is very similar to a pathway recently identified by He and Schmid 69,71

**Hydration **
**solvent **

**(a1) ****t****=10800****τ**** (a2) ****t****=14000****τ**** ****(a3) ****t****=14400****τ**** (a4) ****t****=16400****τ**** (a5) ****t****=23600****τ**** **

**(a6) ****t****=24800****τ**

**(b1) ****t****=10800****τ**** (b2) ****t****=10960****τ**** ****(b3) ****t****=11040****τ**** (b4) ****t****=11200****τ**** (b5) ****t****=11360****τ**

**(c1) ****t****=14400****τ**** (c2) ****t****=14560****τ**** (c3) ****t****=14840****τ**** ****(c4) ****t****=15120****τ**

**Figure 6 **(a) Representative snapshots during the process of
vesicle formation via a platelet intermediate in the absence of
hydrodynamics. (b) Snapshots during the vesicle formation in
the presence of hydrodynamics. The convective flows have

been turned on at time 10800*τ*. (c) Same as (b), but the

convective flows are turned on at time 14400*τ*. The shear

viscosity and bulk viscosity are η*s=*0.22η* and η*b=*0.34η*,

respectively.

from diffusion-only simulations. He et al used
external potential dynamics84_{, which is a dynamic }

SCF model with a non-local kinetic coupling
coefficient that accounts for chain connectivity at the
Rouse level. Like in the present study, the pathway
of He et al. involves micelle growth at early times
and a semi-vesicle intermediate state. However,
coalescence and fusion events were much less
prominent, i.e., the micelle and vesicle growth were
mainly driven by attracting single copolymers from
solution. This difference can partly be attributed to
the different kinetic model (as will be discussed
further below), and partly to the higher copolymer
concentration in the present study. Indeed, when
looking at higher copolymer concentrations in their
model, He et al found a different pathway that
involved micelle coalescence71_{: The micelles }

aggregated into flat bilayer disks which then curved around and closed up to form vesicles. The same mechanism had been observed in previous simulations by other authors 57,58,59 and is also occasionally found here in the diffusion-only simulations (an example of a bilayer intermediate is marked by an arrow in Figure 4, a3). It is not observed in the simulations with convective flow.

To elucidate the influence of hydrodynamic flows on this “disk pathway”, we have carried out a set of simulations where convective flows are turned on at different stages of the vesicle formation process. The results are shown in Figure 6. The upper row (Figure 6a) shows the reference simulation, simulated within

**(a1) ****t****=10800****τ**** (a2) ****t****=12640****τ**** (a3) ****t****=14000****τ**** ****(a4) ****t****=15560****τ**** ****(a5) ****t****=21280****τ**

**(b1) ****t****=10800****τ**** (b2) ****t****=11160****τ**** (b3) ****t****=11240****τ**** ****(b4) ****t****=11280****τ**** ****(b5) ****t****=13280****τ**

**Figure 7 ** Representative snapshots during the fusion process of
two small vesicles (a) in the absence and (b) presence of
hydrodynamic effects. In panel (a), the convective flows are

switched off at time 10800*τ*.

the diffusion-only model. At early stages, spherical micelles coalesce to form cylindrical micelles as above. The cylindrical micelle subsequently transforms itself into a flat bilayer platelet. The platelet merges with neighbour micelles and grows further into a curved disk. Then, the solvent is gradually encapsulated to reduce the energy contribution from the line tension of the rim. This results in a cuplike vesicle with a small pore. Eventually, the pore closes up and a vesicle is formed.

Starting from this diffusion-only simulation, we have investigated the effect of switching on convective flows at different times. The results depend crucially on whether this happens before or after the bilayer disks have formed. In the first case, the disk formation is prevented and the vesicle formation proceeds via the semi-vesicle pathway (Figure 6b). In the second case, the pathway of vesicle formation is similar to that found without hydrodynamic flows, but the rate of pore closure is remarkably sped up by the convective flows (Figure 6c). Thus we conclude that the convective flows not only accelerate the formation of vesicles, but also contribute to selecting the pathway of vesicle formation, and that they favor the semi-vesicle pathway.

10800*τ*, the two small vesicles are separated. Then
the amphiphilic block copolymers in the outer layers
of the vesicles rearrange locally and bridge the
solvent gap between the vesicles. This results in the
formation of a stalk (snapshots a2 and b2).
Subsequently, the stalk intermediate expands and the
outer layers of vesicles recede. The inner layers of
vesicles merge and produce a hemifusion diaphragm
(snapshots a3 and b3). Finally a fusion pore appears
(snapshots a4 and b4). At this time, the fusion
process of vesicles is completed. The freshly formed
vesicle retracts toward a spherical shape, but the rate
of retraction is very slow (snapshots a5 and b5). The
same mechanism is observed both in the absence and
presence of convective flows (Figure 7a and b).
However, the long-range hydrodynamic interactions
accelerate the process by an order of magnitude. The
total time of vesicle fusion takes about 2920*τ* in the
diffusion-only model (from snapshot a2 to a4), and
120*τ* in the presence of hydrodynamics (from
snapshot b2 to b4).

We should note that fusion events were much
more frequent in the present study than in the
previous studies by He et al70,71,72, even in the
diffusive case. This is most likely an artefact of the
local dynamic SCF approach chosen in the present
study. As mentioned above, He et al used external
potential dynamics84_{, which is a dynamic SCF theory }

with nonlocal mobility coefficient that accounts for the chain connectivity. Fusion events practically never occurred in the later stages of the simulations once the vesicles were fully developed. This is consistent with experiments where spontaneous fusion events are practically never observed. In contrast, Sevink and Zvelindovsky 67,68 observed fusion and aggregation in their studies of compact copolymer vesicles in solution, much like in the present study. They also used a local version of dynamic SCF theory.

To conclude our analysis of hydrodynamic effects on vesicle formation, we will now examine a number of quantities that characterize the vesicle configurations at a global level. One highly relevant quantity is the solvent content inside the vesicles. Figure 8 shows the volume fraction of trapped solvent as a function of time during the evolution process of the aggregates. The trapped solvent is confined in the inner layers of vesicles and consists of the hydration solvent of the inner leaflets and the interior bulk solvent, which were illustrated in Figures 5d and 5e, respectively. The volume fraction

**0** **10000** **20000** **30000** **40000**

**0.00**
**0.02**
**0.04**
**0.06**

**0.08** **diffusion only**

η

**s/**η

∗

**=0.36**

η** _{s}/**η∗

**=0.22**

**f****tra**

**p**

**Time/**τ

**Figure 8 **Total volume fraction of trapped solvent as a function
of time for the self-assembly of amphiphilic block copolymers.
In the calculations, the trapped solvent consists of the interior
bulk solvent and hydration solvent in the inner layers of
vesicles, as illustrated in Figures 5e and 5d.

of trapped solvent is given by f*trap*=V*tra*p/V*tot*, where
*Vtra*p and Vtot are the volume of the trapped solvent

and the total solvent in the system, respectively. In the early stages of aggregation, where the amphiphilic block copolymers are still mainly organized in micelles and semi-vesicles, the amount of trapped solvent is small. At this stage, the error bars are quite small, indicating that there is little statistical spread in the amount of trapped solvent: As long as most of the trapped solvent is hydration solvent, its volume fraction is closely linked to the distribution of A and B blocks in the aggregates and there is little room for variations. This changes as soon as the semi-vesicles begin to fill with interior bulk solvent, which happens around ftrap~0.006. The error bars increase dramatically and the amount of trapped solvent rises, first linearly up to ftrap~0.06, and then slowly saturating. In the presence of hydrodynamic flows, this process sets in earlier and proceeds considerably faster than in the absence of hydrodynamics.

**0** **10000** **20000** **30000** **40000**
**0.20**

**0.25**

**diffusion only**

η** _{s}/**η∗

**=0.36**

η** _{s}/**η∗

**=0.22**

**(a)**

**V/**

**L**

**3**

**Time/**τ

**0** **10000** **20000** **30000** **40000**
**5**

**10**
**15**
**20**

**(b)**

**A/**

**L**

**2**

**Time/**τ

**0** **10000** **20000** **30000** **40000**

**0**
**30**
**60**
**90**
**120**

**(c)**

**2**

**H/L**

**Time/**τ

**0** **10000** **20000** **30000** **40000**
**0**

**60**
**120**
**180**
**240**

**20000** **30000** **40000**
**10**

**20**
**30**
**40**

A
**(d)**

χ**E**

**/2**

**Time/**τ

**Figure 9** Temporal evolutions of the Minkowski functionals for
the hydrophobic B-beads during the quenching process of
amphiphilic block copolymers with and without hydrodynamic
effects. Panels (a), (b), (c), and (d) respectively show the

volume (*V*), area (*A*), integral mean curvature (*H*), and Euler

characteristic (*χE*). *L* is the size of simulation box. The inset of

panel (d) shows the Euler characteristic as a function of time in the late stage.

value of 2, and that of hollow spheres has a value of 4. The Euler characteristic of systems containing disjoint objects is equal to the sum of Euler characteristic of the individual objects. If two objects are linked by a passage, the Euler characteristic changes by (-2).

qualitative effect on the global morphological evolution of the system.

**4. DISCUSSION AND CONCLUSION**

To summarize, we have introduced a new method to treat hydrodynamic interactions in dynamic SCF simulations within a hybrid Lattice-Boltzmann/finite difference scheme, which solves a coupled set of SCF-based convection-diffusion equations and Navier-Stokes equations.

A few comments on the implementation of the
method are in order. First, we have taken care to
include fluctuations both in the convection-diffusion
equations *and in the Navier-Stokes equations. Thus *
we have implemented the fluctuating LB method,
even though it is much less widely applied and
computationally more expensive than regular,
deterministic LB. The reason is that the amplitudes
of the fluctuations in the convection-diffusion
equations and the Navier-Stokes equations are
intimately related. The noise level is basically given
by the inverse of Ω=h3/υ0, which is the number of

beads per lattice voxel. The smaller the number of
beads per lattice point, the larger are the stochastic
forces *both in the discretized versions of the SCF *
equations and the fluctuating LB equations. In a
consistent treatment, one must therefore either
include them everywhere or omit them everywhere.
In practice, however, we found that the treatment of
the noise does not seem to be very critical. For
comparison, we have also run the simulations of
section 3.2 using the deterministic LB scheme (with
noise switched off). The results were virtually
identical to those presented here (data not shown). In
most practical situations, it is thus probably
acceptable to neglect the hydrodynamic noise.
Nevertheless, we believe that such an approach is
problematic from a conceptual point of view, because
different degrees of freedom are coupled to heat
baths of different temperature (T ~300 K for the
composition degrees of freedom, T=0K for the flow
degrees of freedom). This might lead to a constant
unphysical heat flux from one thermal reservoir to
the other and result in simulation artefacts, and even
“violations” of the second law of thermodynamics.

Second, the dynamical model in our implementation is purely local in space and time and does not account for the effects of chain connectivity. For example, the monomer diffusion in Eq. (3) is driven by a local Onsager mobility coefficient. We have discussed in section 3.2 that the chain

connectivity may influence the dynamics, e.g., it
creates a kinetic barrier for fusion events. To
overcome this problem, one can replace Eq. (3) by a
convection-diffusion model based on “external
potential dynamics”84_{, which implements the }

dynamical behavior of Rouse chains. One subtle issue here is to implement the noise both efficiently and in a thermodynamically consistent manner, which can be done, but requires slight (well-motivated) changes in the underlying SCF free energy functional 29,93.

A more serious drawback of the present method
is that it does not correctly account for the
viscoelastic behaviour of dense polymers melts,
unless the viscoelacity results from the microphase
separation itself.94,95 The hydrodynamic constitutive
equations, σ_{αβ} =η_{αβγδ}∂_{γ}*u*_{δ} , describe Newtonian
fluids without memory. Furthermore, the SCF free
energy functional is based on a reference ensemble of
equilibrium polymers and does not include the
possibility of chain stretching in shear flow. Our
method can be refined in both respects. On the one
hand, several approaches have been proposed to
incorporate viscoelastic constitutive equations in LB
simulations.96,97,98,99,100 On the other hand, Maurits et
al101 have devised a heuristic method to incorporate
chain stretching in shear flow by adjusting the
reference ensemble of polymer configurations in the
free energy functional. However, it is not clear how
these different extensions should be combined in a
unified and consistent way. Ideally, the macroscopic
viscoelastic constitutive equation should emerge
from a microscopic simulation model that accounts
for chain stretching and the effect of entanglements
on the diffusive motion of chains. The construction
of such a model is far from trivial.